2D damping predictions of fiber composite plates: Layup effects


 Brittany Webster
 1 years ago
 Views:
Transcription
1 Available online at Composites Science and Technology 68 (2008) COMPOSITES SCIENCE AND TECHNOLOGY 2D damping predictions of fiber composite plates: Layup effects E.K. Billups, M.N. Cavalli * University of North Dakota, Department of Mechanical Engineering, Stop 8359, 243 Centennial Drive, Grand Forks, ND , United States Received 29 November 2006; received in revised form 25 May 2007; accepted 12 September 2007 Available online 20 September 2007 Abstract Several twodimensional theories for predicting the specific damping capacity (SDC) of fiber composite laminates are compared. The theories considered are those of Adams and Bacon, Adams and Maheri, Ni and Adams and Saravanos and Chamis. No interlaminar effects are considered. Results show that the theory of Saravanos and Chamis provides the most consistent fit to experimental results for a range of material properties and laminate layups. For some laminates, however, the Saravanos and Chamis method seems to predict the wrong trend in SDC variation versus layup angle. It is not clear from the current work whether this result is due to the absence of interlaminar effects in the theory or the presence of a threedimensional stress state in the laminate. Ó 2007 Elsevier Ltd. All rights reserved. Keywords: A. Polymer matrix composites; A. Structural materials; B. Modeling; C. Laminate theory 1. Introduction Energy dissipation, or damping, is an important consideration in a variety of engineering designs. Composite materials offer the unique ability to tailor damping behavior, and other properties, for specific applications [1 4]. As a result, composites can be desirable choices in applications as varied as wind turbine blades [5 9], beams and shafts [10,11] and control surfaces [12,13]. A full analysis of damping performance for arbitrary composite structures typically requires threedimensional numerical analysis due to the mathematical complexity of the problem [14 17]. Simplified, twodimensional analyses based on the principles of Classical Laminate Theory (CLT) have shown good agreement for particular materials, layups, and geometries, however [1 4,18]. The goal of the current work is to compare several theories available in the literature for predicting the specific damping capacity (SDC) of composite laminates. Theories of Adams and Bacon [1], Ni and Adams [3], Adams and * Corresponding author. Tel.: ; fax.: address: (M.N. Cavalli). Maheri [18] and Saravanos and Chamis [19,20] will be examined. Results from each theory will be compared with experimental measurements of SDC values. These comparisons will help illustrate the strengths and shortcomings of each theory as well as the use of twodimensional damping predictions generally. An example will then be presented of how the Saravanos and Chamis method can be applied to a composite beam whose plies are assembled at arbitrary angles. Damping, stiffness and deflection predictions for this arbitrary laminate will be presented graphically in several forms, each with specific advantages in terms of selecting a layup for a particular set of design requirements. This example will illustrate the usefulness of the technique in designing fiber composite structures. 2. Theory 2.1. Overview All theories compared in this work are based on the assumptions of classical laminate theory for orthotropic materials [21,22]. In short, this implies perfect bonding between plies, no out of plane stresses or strains and small, /$  see front matter Ó 2007 Elsevier Ltd. All rights reserved. doi: /j.compscitech
2 728 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) elastic deformations [21,22]. Matrices of applied forces and moments are written as [N] and [M], respectively, with subscripts used to indicate specific components. The typical notation used in this paper for subscripts, unless otherwise noted, is number subscripts, i.e. 1, 2, or 12, are used to denote principal material directions of a lamina while letter subscripts, i.e. x, y, orxy, denote the global coordinates of the laminate. The two coordinate systems are typically offset by an angle, h. For elastic deformations, the strain energy stored in each ply can be separated into three components: strain energy in the fiber direction, strain energy transverse to the fiber direction, and strain energy in shear. Some amount of each of these components is dissipated during deformation. One way to quantify this dissipation is by using the specific damping capacity which is defined as the strain energy dissipated during a stress cycle, DU, divided by the maximum strain energy during a stress cycle, Eq. (1). w ¼ DU ð1þ U max The total strain energy dissipated for each lamina is the product of the lamina strain energy components with the damping coefficient for the appropriate mode of deformation, all integrated over the thickness of the ply. Consequently, this method requires knowledge of three damping coefficients for each lamina: the longitudinal (fiber direction) coefficient, w Lk, the transverse coefficient, w Tk, and the inplane shear coefficient, w LTk, where the subscript k denotes these are the properties of the kth lamina. The damping coefficients can be determined via tests on unidirectional laminates under various angles of loading. The energy dissipation can be summed over the total number of plies and, using the total energy dissipated in the laminate, the overall specific damping capacity (SDC) written as [1]: w laminate ¼ w 1 þ w 2 þ w 12 ð2þ 2.2. Adams and Bacon theory Adams and Bacon [1] presented a general equation to predict the SDC of beams for applied forces, {N}, and moments, {M}. The equation can be used for any laminate configuration and the lamina damping coefficients (w Lk, w Tk, w LTk ) are allowed to be stress dependent: w laminate ¼ 2P n R hk h k 1 ðdðdu 1 ÞþdðDU 2 ÞþdðDU 12 ÞÞdz fng T fe o gþfmg T fjg ð3þ Eq. (3) includes contributions from all inplane stresses but does not allow for outofplane contributions to energy dissipation. The latter limitation is consistent for all theories presented in this paper. The number of terms involved in Eq. (3) leads to a level of complexity that can typically only be handled using numerical techniques. Adams and Bacon recognized this and derived several approximations to Eq. (3) that lend themselves to easier solutions by neglecting certain stresses and strains or limiting the allowable layups [1] Ni and Adams theory Additional damping prediction equations were developed by Ni and Adams [3]. They assumed free flexure deformation, stressindependent damping coefficients and a symmetric layup [3]. This final assumption leads to no midplane strains under classical laminate plate theory. In addition to neglecting r y and s xy, Ni and Adams also argued that the transverse strain, e y, in each lamina will be much smaller than the longitudinal and shear strains and could be neglected [3], resulting in Eqs. (4) (6) w 1 ¼ 8w X p=2 L m 2 ðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ðm 2 C 11 þ mnc 16 ÞW k ð4þ w 2 ¼ 8w X p=2 T n 2 ðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ðn 2 C 11 mnc 16 ÞW k ð5þ w 12 ¼ 8w X p=2 LT mnðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ð2mnc 11 m 2 n 2 C16 ÞW k ð6þ where [C] is the normalized flexural compliance of the laminate, [Q k ] is the stiffness of the kth lamina, p is the total number of plies present in the laminate and W k is a weighting factor based on the position of the kth lamina within the laminate [3] Adams and Maheri theory Revisions to the Ni and Adams equations were made by Adams and Maheri [18]. The derivation of the equation deviated from the method used by Ni and Adams but the final result is similar. In short, the Adams and Maheri theory is the Ni and Adams theory with slight notational changes and the transverse lamina strain, e y, term included [18] Saravanos and Chamis theory The expression for the strain energy of a general laminate under general loading has been formulated by Tse and Lai [23] and Saravanos and Chamis [19]. Saravanos and Chamis have also written the three SDC components in matrix form [19,20]. These results can be combined to give an expression for the SDC of an arbitrary laminate under general loading which can be written as
3 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) T N A B T A D B D A B N M C D B w laminate ¼ D D D C D M T N A B T ð7þ N M C D M where A *, B *, C * and D * represent the components of the inverse of the original material stiffness matrix [21,22]. A D, B D, C D and D D are the components of the original stiffness matrix multiplied by appropriate damping coefficients. Eq. (7) is the basis of the Saravanos and Chamis theory. It should be noted that in their original work, Saravanos and Chamis also include the possibility of interlaminar effects, but those are not considered here [21,22]. Though it is not perhaps immediately apparent, the form of the Saravanos and Chamis theory expression for laminate damping is very similar in form to that previously developed by Adams and Bacon (Eq. (3)). An important distinction is that Eq. (7) is written in terms of stiffnesses and strains while Eq. (3) is written in terms of stresses and compliances. This made sense for Adams and Bacon because they included stressdependence in their damping coefficients which the Saravanos and Chamis theory does not. The tradeoff, however, is that the Adams and Bacon form is less computationally efficient. 3. Results and discussion 3.1. Comparison with previous work Experimentally determined values for the specific damping coefficients were obtained from the literature for several variations of Eglass epoxy and carbon epoxy fiber composites under freefree flexural loading [1 3]. Table 1 lists the material properties for each laminate [1 3]. These values were used in the Ni and Adams [3], Adams and Maheri [2] and Saravanos and Chamis [19] theories to calculate the predicted values of SDC for various fiber geometries. All calculations were performed using MATLAB (The Mathworks, Natick, MA). Unfortunately, the general theory of Adams and Bacon can only be compared with the data presented in the original paper [1]. This is because the theory allows for stress dependent damping coefficients but does not explicitly identify the relationship between the coefficients and the lamina stresses. The results of Adams and Bacon could thus not be recalculated for other laminate geometries. Transcription of data points from the original plots has been used to recreate their curves in the current work. Adams and Maheri [2] measured the specific damping capacity of two laminate configurations of Fibredux 913/ glass fiber composites. The first was a balanced symmetric angleply laminate, [ h /+h / h /+h ] s and the second was a symmetric unidirectional laminate, [h ] 8. Beams were cut from plates with the above layups and excited at the fundamental flexural mode of vibration. The variation of the SDC with fiber orientation for these configurations is shown in Figs. 1 and 2, respectively. Note that results from two beam widths are plotted in Fig. 1. No experimental uncertainty is presented with the original data, but the beam width does not appear to cause a dramatic effect on the damping [2]. Results from Kyriazoglou and Guild indicate this may not be the case for larger ranges of aspect ratios [24]. All theories predict the SDC values reasonably well for both laminates. The blank legend symbol for the Adams/Maheri theory indicates that this theory is identical to the theory listed above it (Saravanos, in this case) for this particular laminate. Figs. 3 and 4 show results from experiments conducted by Adams and Bacon [1] on DX209/carbon fiber composite laminates. The layup in Fig. 3 is [h] 10 and the layup in Fig. 4 is [+h/ h] 5. No information is given regarding the difference between experimental data sets 1 and 2 in Fig. 3 [1]. The Sarvanos and Chamis theory and the Adams and Bacon theory provide the most consistent fit in terms of both magnitude of the predicted SDC and shapes of the curves. Fig. 4 shows that there are some layup/material Table 1 Material properties for damping results presented. Material E 1 (ksi GPa) E 2 (ksi GPa) G 12 (ksi GPa) m 12 w L (%) w T (%) w LT (%) V f References Fiber Matrix Eglass Epoxy (DX 210) [3] Eglass Epoxy (Fibredux 913) [2] HMS carbon Epoxy (DX 209) 27, [1] HMS carbon Epoxy (DX 210) 25, [3]
4 730 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Fig. 1. Variation of the specific damping capacity with fiber orientation for a glass/epoxy (Fiberdux 913G) laminate with a symmetric angleply layup of [ h /+h / h /+h ] s. Fig. 4. Variation of the specific damping capacity with fiber orientation for carbon/epoxy (HMS/DX209) laminate with a angle ply layup of [+h / h ] 5. Fig. 2. Variation of the specific damping capacity with fiber orientation for a glass/epoxy (Fiberdux 913G) laminate with a unidirectional layup of [h ] 8.. combinations where the 2D theories are not able to fully predict the behavior of the material. This may be due to interlaminar effects or may indicate that a threedimensional stress state exists for this laminate. Since no uncertainty is quoted on the experimental data, however, no firm conclusion can be reached. Ni and Adams [3] investigated symmetric laminates, [h /(h + 90) /(h + 45) /(h 45) ] s, for both glass and carbon fibers with DX210 epoxy. The widthtolength ratios of the beams used in the experimental damping determination was 1:17. The variation of the SDC with respect to the outer ply orientation for a glass and carbons composites is shown in Figs. 5 and 6, respectively. The damping trend is captured reasonably well by all theories for the glass fiber composite but significant discrepancies are apparent for the carbon fiber material. Both the Adams and Maheri and Ni and Adams theories significantly overpredict the damping for positive angles and neither capture the shape of the SDC curve for positive Fig. 3. Variation of the specific damping capacity with fiber orientation for carbon/epoxy (HMS/DX209) laminate with a unidirectional layup of [h ] 10. Fig. 5. Variation of the specific damping capacity with outer ply fiber orientation for a glass/epoxy (glass/dx210) laminate with a layup of [h / (h + 90) /(h + 45) /(h 45) ] s.
5 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) of w 2 are positive for all orientations in the Ni and Adams and Saravanos and Chamis theories but the shapes of the two curves are significantly different. These differences can be traced back to the fundamentally different assumptions regarding stresses and strains within the plies Predictions of damping for arbitrary laminates Fig. 6. Variation of the specific damping capacity with outer ply fiber orientation for a carbon/epoxy (HMS/DX210) laminate with a layup of [h /(h + 90) /(h + 45) /(h 45) ] s. values of h as well as the Saravanos and Chamis theory. For negative values of h, both Adams and Maheri and Ni and Adams again overpredict the measured damping. The Saravanos and Chamis theory gives reasonable predictions for the SDC magnitude at negative values of h, but seems to predict the wrong shape for the SDC curve near h ¼ 45. It is not clear if the discrepancies between the theory and data for this laminate arise from uncertainty in the experimental results, edge effects, interlaminar effects or a threedimensional stress state. Fig. 7 shows an interesting result for the Adams and Maheri theory applied to the [h /(h + 90) /(h + 45) / (h 45) ] s carbon/dx210 laminate. The w 2 component of the SDC is plotted versus outer ply orientation. For some orientations, the Adams and Maheri theory actually predicts negative values of w 2, an unrealistic result that implies energy generation, rather than damping. Values The Saravanos and Chamis theory will now be applied to an arbitrary laminate to illustrate the information that can be provided regarding composite laminate properties. Values from Table 1 for the Ni and Adams Fibredux 913/glass fiber damping coefficients will be used for all predictions [3]. The laminate to be analyzed is of the form [h 1 / (h 1 + a) /(h 1 a) /(h 1 + a) / (h 1 a) / (h 2 a) / (h 2 + a) / (h 2 a) / (h 2 + a) / h 2 ], where h 1, h 2, and a could take on any value from 0 to 180. First, let us select a single value for the offset angle, a ¼ 90. Fig. 8 illustrates how the SDC of the resulting laminate varies with changes in h 1 and h 2 under M x loading. The maximum possible value of SDC is approximately 5.7% and occurs when h 1 ¼ 48 and h 1 ¼ 132. Note that the resolution of Fig. 8 for both h 1 and h 2 is 2. The minimum level of damping that can be achieved in this laminate is about 1.7%, when h 1 ¼ h 2 ¼ 90. Referring to Table 1, most energy in this material is dissipated by deformations in the matrix, so both of these results make sense. Values of h 1 and h 2 near 45 result in a large contribution from matrix deformation and lead to large overall values of energy dissipation. In contrast, values of h 1 and h 2 near 90 result in most of the laminate (8 of 10 plies) having Fig. 7. Variation of the specific damping capacity component w 2 with outer ply fiber orientation for a carbon/epoxy (HMS/DX210) laminate with a layup of [h /(h + 90) /(h + 45) /(h 45) ] s. Fig. 8. Variation of SDC (%) prediction with fiber orientation angle for glass/epoxy in a symmetric layup of [h 1 /(h ) /(h 1 90) /(h ) / (h 1 90) /(h 2 90) /(h ) /(h 2 90) /(h ) /h 2 ] for M x 5 0.
6 732 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Fig. 9. Variation of SDC (%) prediction with fiber orientation angle for glass/epoxy in a symmetric layup of [h 1 /(h ) /(h 1 90) /(h ) / (h 1 90) ] s for M x 5 0. the fiber direction aligned along the xaxis. This leads to very little damping contribution from matrix deformations and minimizes the overall energy dissipation. It is necessary to recognize that the value of the SDC may not be the only laminate property of interest. If a laminate deforms in an undesirable way during loading or curing (e.g. warps), it may not be able to fulfill its design requirements despite desirable energy dissipation characteristics. Similarly, the laminate must possess the proper effective stiffness under a given mode of loading. Contours showing laminate effective stiffness and warpage behavior as a function of layup geometry can be created easily by incorporating the appropriate equations into the MATLAB code. These can then be compared with the SDClayup contour (Fig. 8) to optimize the composite layup. It is possible that the entire design space of Fig. 8 is not attainable or desirable in a given manufacturing situation. The simplicity of a symmetric layup may be desirable, for example. In such a situation, a second method of analyzing the Saravanos and Chamis theory results would be to pull out SDC values along a specified section of Fig. 8. For a symmetric laminate, Fig. 9 is the result. Fig. 9 indicates that values of h 1 must be between 31 and 59 to achieve damping within about 10% of the maximum value for a symmetric laminate. To be within about 10% of the minimum value, h 1 must be between 85 and 95. Corresponding sections could be constructed for various conditions (h 1 ¼ constant, h 2 ¼ constant, h 1 / h 2 ¼ constant, etc.). A third method of using the Saravanos and Chamis technique is to allow all angles, h 1, h 2, and a, to vary from 0 to 180. This method allows the full range of laminate properties that can be achieved to be identified. Fig. 10 shows the range of SDC that are predicted for this laminate as a function of the effective flexural stiffness. The maximum achievable value of SDC is approximately 6% and occurs in a laminate with h 1 ¼ h 2 ¼ 48 and a ¼ 0. Minimum damping (0.8%) occurs in a laminate with h 1 ¼ h 2 ¼ a ¼ 0. The fact that the maximum damping is Fig. 10. SDC flexural modulus envelope showing all possible combinations predicted by CLT theory for glass/epoxy laminate with layup [h 1 /(h 1 + h) /(h 1 h) /(h 1 + h) /(h 1 h) /(h 2 h) /(h 2 + h) /(h 2 h) / (h 2 + h) /h 2 ]. in a layup of approximately ±45 and the minimum damping is in the stiffest laminates is not surprising given the material properties. What makes Fig. 10 interesting is the fact that it clearly shows that for a given value of effective stiffness, it may be possible to tailor the SDC of the laminate over a relatively large range. Similar design envelopes can be defined for other types of loadings as well as laminate outofplane deformations. The calculations required to construct Fig. 10 resulted in approximately 26,000 data points and required approximately 45 minutes to complete on a 3GHz Pentium 4 PC. With the information from the CLT method presented in this form, damping, stiffness and warpage of potential laminates can be quickly assessed. 4. Conclusions A comparison of the damping predictions from several twodimensional composite laminate theories has been conducted. Results indicate that the general theory of Saravanos and Chamis most consistently agrees with experimental results. Certain layup/material combinations show significant deviations between theoretical predictions and experimental data, particularly with stiffer carbon reinforcement. More work is needed to determine whether these differences arise from interlaminar, edge or threedimensional stress effects. The Saranavos and Chamis method has been used to predict the damping, stiffness and outofplane deformation for an arbitrary composite laminate. Several approaches to the analysis are presented to quickly identify the performance envelope of a specific laminate and to tailor properties such as the specific damping coefficient (SDC) and the effective stiffness. These approaches could be applied to structures such as wind turbine blades where energy dissipation and stiffness both play a large role in successful design performance.
7 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Acknowledgement Financial support of Mr. Billups from the UND Mechanical Engineering Department during the course of this work is gratefully acknowledged. References [1] Adams RD, Bacon DGC. Effect of fibre orientation and laminate geometry on the dynamic properties of CFRP. J Compos Mater 1973;7: [2] Adams RD, Maheri MR. Dynamic flexural properties of anisotropic fibrous composite beams. Compos Sci Technol 1994;50(4): [3] Ni RG, Adams RD. The damping and dynamic moduli of symmetric laminated composite beams theoretical and experimental results. J Compos Mater 1984;18(2): [4] Chandra R, Singh SP, Gupta K. Damping studies in fiberreinforced composites a review. Compos Struct 1999;46: [5] Bechly ME, Clausen PD. Structural design of a composite wind turbine blade using finite element analysis. Comput Struct 1999;63(3): [6] Lobitz D, Veers PS, Migliore PG. Enhanced performance of HAWTs using adaptive blades. In: Proceedings of the wind 1996 ASME wind energy symposium. Houston, Texas, USA: ASME; [7] Lee AT, Flay RGJ. Compliant blades for wind turbines. The Inst Prof Eng New Zealand 1999;26(1):7 12. [8] Garfinkle M. Twisting smartly in the wind. Aerospace Amer 1994;32(7): [9] Chandra R. Active shape control of composite blades using shape memory actuation. Smart Mater Struct 2000;10(5): [10] Bert CW, Kim C. Whirling of compositematerial driveshafts including bendingtwisting coupling and transverse shear deformation. J Vibr Acoust 1995;117(1): [11] Lentz WK, Armnaios EA. Optimum coupling in thinwalled, closedsection composite beams. J Aerospace Eng 1998;11(3):81 8. [12] Klous H, Mirza S. Piezoelectric induced bending and twisting of laminated composite shallow shells. Smart Mater Struct 2000;9(4): [13] Kim C, Park BS, Goo NS. Shape changes by coupling bending and twisting of shapememoryalloyembedded composite beams. Smart Mater Struct 2002;11(4): [14] Wetherhold RC, Panthalingal N. Piezoelectric PZT/epoxy composites for controlling torsional motion. J Intell Mater Syst Struct 1994;5: [15] Chandra R, Singh SP, Gupta K. A study of damping in fiberreinforced composites. J Sound Vibr 2003;262: [16] Hwang SJ, Gibson RF. The effects of threedimensional states of stress on damping in laminated composites. Compos Sci Technol 1991;41: [17] Hwang SJ, Gibson RF. Influence of bendingtwisting and extensionbending coupling on damping of laminated composites. J Mater Sci 1993;28:1 8. [18] Adams RD, Maheri MR. Damping in advanced polymer matrix composites. J Alloys Comp 2003;355(1 2): [19] Saravanos DA, Chamis CC. Unified micromechanics of damping for unidirectional fiber reinforced composites, NASA TM National Aeronautics and Space Administration, Cleveland; [20] Saravanos DA, Chamis CC, Mechanics of damping for fiber composite laminates including hygrothermal effects, NASA TM National Aeronautics and Space Administration, Cleveland; [21] Jones RM. Mechanics of composite materials. Philadelphia: Taylor & Francis; [22] Kaw AK. Mechanics of composite materials. Boca Raton, Florida: CRC Press; [23] Tse PC, Lai TC. Expression for the strain energy of laminated composite thin shells. Int J Mech Eng Educ 1995;23(2): [24] Kyriazoglou C, Guild FJ. Finite element prediction of damping of composite GFRP and CFRP laminates a hybrid formulation vibration damping experiments and Rayleigh damping. Compos Sci Technol 2006;66(3 4):
Passive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationThermal Vibration of Magnetostrictive Material in Laminated Plates by the GDQ Method
The Open echanics Journal, 007, 1, 937 9 Thermal Vibration of agnetostrictive aterial in Laminated Plates by the GDQ ethod C.C. Hong * Department of echanical Engineering, Hsiuping Institute of Technology,
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationFREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR THIN PLATES EMBEDDED WITH SHAPE MEMORY ALLOY FIBERS
Journal of Thermal Stresses, 33: 79 96, 2010 Copyright Taylor & Francis Group, LLC ISSN: 01495739 print/1521074x online DOI: 10.1080/01495730903409235 FREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationNonlinear Transient Response of Basalt/Nickel FGM Composite Plates under Blast Load
Nonlinear Transient Response of Basalt/Nickel FGM Composite Plates under Blast Load Baştürk, S., Uyanık, H., & Kazancı, Z. (2016). Nonlinear Transient Response of Basalt/Nickel FGM Composite Plates under
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationNONLINEAR DYNAMIC ANALYSIS OF AN ORTHOTROPIC COMPOSITE ROTOR BLADE
Journal of Marine Science and Technology, Vol., o. 4, pp. 4755 (4) 47 OIEAR DYAMIC AAYSIS OF A ORTHOTROPIC COMPOSITE ROTOR BADE MingHung Hsu Key words: orthotropic composite rotor blade, differential
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationINTRODUCTION TO PIEZO TRANSDUCERS
PIEZO SYSTEMS, INC. 65 Tower Office Park Woburn, MA 01801 USA Tel: 781 933 4850 Fax: 781 933 4743 email: sales@piezo.com Find Search for a product or category HOME PRODUCTS CUSTOM OEM CATALOG TECHNICAL
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationVIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES. 1. Introduction
ARCHIVES OF ACOUSTICS 31, 4 (Supplement), 53 58 (2006) VIBRATION ENERGY FLOW IN WELDED CONNECTION OF PLATES J. CIEŚLIK, W. BOCHNIAK AGH University of Science and Technology Department of Robotics and Mechatronics
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationMatrix cracking in polymeric composites laminates: Modelling and experiments
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 230 237 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech Matrix cracking in polymeric composites
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationRELIABILITYBASED DESIGN AND OPTIMIZATION OF SELFTWISTING COMPOSITE MARINE ROTORS
Proceedings of the ASME 28th International Conference on Ocean, Offshore and Arctic Engineering OMAE29 May 3June 5, 29, Honolulu, Hawaii OMAE29867 RELIABILITYBASED DESIGN AND OPTIMIZATION OF SELFTWISTING
More informationDue Monday, September 14 th, 12:00 midnight
Due Monday, September 14 th, 1: midnight This homework is considering the analysis of plane and space (3D) trusses as discussed in class. A list of MatLab programs that were discussed in class is provided
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More informationPiezoelectric Composites as Bender Actuators
Integrated Ferroelectrics, 71: 221 232, 2005 Copyright Taylor & Francis Inc. ISSN 10584587 print / 16078489 online DOI: 10.1080/10584580590964673 Piezoelectric Composites as Bender Actuators Karla Mossi,
More informationVIBRATION ANALYSIS OF EULER AND TIMOSHENKO BEAMS USING DIFFERENTIAL TRANSFORMATION METHOD
VIBRATION ANALYSIS OF EULER AND TIMOSHENKO BEAMS USING DIFFERENTIAL TRANSFORMATION METHOD Dona Varghese 1, M.G Rajendran 2 1 P G student, School of Civil Engineering, 2 Professor, School of Civil Engineering
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More informationFree Vibration Analysis of Kirchoff Plates with Damaged Boundaries by the Chebyshev Collocation Method. Eric A. Butcher and Ma en Sari
Free Vibration Analysis of Kirchoff Plates with Damaged Boundaries by the Chebyshev Collocation Method Eric A. Butcher and Ma en Sari Department of Mechanical and Aerospace Engineering, New Mexico State
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationEFFICIENT DETERMINATION OF MECHANICAL PROPERTIES OF CARBON FIBREREINFORCED LAMINATED COMPOSITE PANELS
EFFICIENT DETERMINATION OF MECHANICAL PROPERTIES OF CARBON FIBREREINFORCED LAMINATED COMPOSITE PANELS Umar Farooq and Peter Myler Faculty of Engineering and Advanced Sciences, University of Bolton BL3
More informationModeling of Interphases in FiberReinforced Composites Under Transverse Loading Using the Boundary Element Method
Y. J. Liu 1 Assistant Professor, email: Yijun.Liu@uc.edu Mem. ASME N. Xu Graduate Student Department of Mechanical, Industrial, and Nuclear Engineering, P.O. Box 210072, University of Cincinnati, Cincinnati,
More informationTHE EFFECT OF FIBER ORIENTATION AND LAMINATE STACKING SEQUENCES ON THE TORSIONAL NATURAL FREQUENCIES OF LAMINATED COMPOSITE BEAMS
IJRET: International Journal of Research in Engineering and Technology eissn: 3191163 pissn: 317308 THE EFFECT OF FIBER ORIENTATION AND LAMINATE STACKING SEQUENCES ON THE TORSIONAL NATURAL FREQUENCIES
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationBilinear Quadrilateral (Q4): CQUAD4 in GENESIS
Bilinear Quadrilateral (Q4): CQUAD4 in GENESIS The Q4 element has four nodes and eight nodal dof. The shape can be any quadrilateral; we ll concentrate on a rectangle now. The displacement field in terms
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationDevelopment and characterization of a rotary motor driven by anisotropic piezoelectric composite laminate
Smart Mater. Struct. 7 (1998) 327 336. Printed in the UK PII: S09641726(98)912289 Development and characterization of a rotary motor driven by anisotropic piezoelectric composite laminate SW Ricky Lee
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More information